International Journal of Engineering Research Volume No.3, Issue No.1, pp : 21-25

(ISSN:2319-6890)(online),2347-5013(print) 01 Jan. 2014

Prediction of Mechanical Properties of Hybrid Fiber Reinforced Polymer Composites P Sivaraj, G Rajeshkumar Theni Kammavar Sangam College of Technology, Theni – 625534, Tamil Nadu, India Email : sivis87@gmail.com, rajesh.mech022@gmail.com Abstract— This work presents a systematic approach to evaluate and study the effect of process parameters on tensile flexural and impact strength of coir and bagasse fiber reinforced polyester-based hybrid composites and also predicts the properties of random oriented hybrid composites. The composite panel was fabricated using hand lay-up method to the size of 300mmx200mmx3mm with various weight percentage of natural fibers namely coir (10, 20 and 30 wt %) and bagasse (10, 20 and 30 wt %) combined with polyester resin. The mechanical properties testing such as tensile, flexural and impact strength were carried out for the samples cut from the fabricated composite panel to the dimensions as per ASTM standard. The significant contribution of mixing of fiber was determined by analysis of variance. The second-order polynomial curve fitting equations are modelled to predict the mechanical properties such as tensile, flexural and impact strength. Also scanning electron microscopy testing was conducted on tensile test specimen to find the fiber matrix interfacial adhesion. Keywords— Hybrid fibers, polyester, tensile strength, flexural strength, impact strength, ANOVA, SEM.

I. Introduction Natural fibers are hair like material which is directly obtained from an animal, vegetable, or mineral source and convertible into nonwoven fabrics such as felt or paper or, after spinning into yarns, into woven cloth. In this research coir and bagasse were used as natural fibers and the polyester as resin material. Coir fiber is obtained from the Outer layer of the fruit of Coconut tree (Cocos Nucifera L). This outer layer is called the coconut husk. The husk (exocarp) of the coconut consists of a smooth waterproof outer skin (epicarp) and fibrous zone (mesocarp). The mesocarp comprises of strands of fibro vascular bundles of coir embedded in a non fibrous paranchymatous "corky" connective tissue usually referred to as pith; which ultimately becomes coir dust. Bagasse, also called Megass, fiber remaining after the extraction of the sugarbearing juice from sugarcane. The word ‘bagasse’, from the French ‘bagage’ via the Spanish ‘bagazo’, originally meant ‘rubbish’, ‘refuse’, or ‘trash’. The chemical name of polyester resin is 1,3-Benzene dicarboxylic acid, polymer with 1,4cyclohexane dimethanol, 2,2-dimethyl-1, 3-propanediol and IJER@2014

2,5-furandione. Its molecular formula is (C8H6O2, C8H16O4, C5H12O2, C4H2O3)n. Ambient temperature cure unsaturated polyester resins provide the ability to produce high-quality, value added composite products. In recent years, hybrid composites containing two or more fibers obtained considerable attention. Natural fibers are renewable, cheaper, support no health hazards and finally provide a solution to environmental pollution by finding new uses for waste materials.

II. Materials and Methods In this investigation the coir and bagasse fibers were taken to reinforce with the polyester resin. Chemical treatment After the fibers were collected, the coir was allowed to undergo with the chemical treatment by using the 6-8% of NaOH with the distilled water. This treatment was used to remove the lignin content in the fiber. The lignin content may affect the Young’s modulus of the fiber. So, the fiber was treated by using the NaOH. Mould preparation To prepare the composite, polyester resin was used as matrix material. The chopped coir and bagasse fibers hybrid composite sheets were manufactured by simple hand lay-up process in a mould. The mould was prepared to fabricate the test specimen. The dimensions of the mould were 300mmx200mmx3mm. Nine hybrid composites with different combinations of coir fiber content (10, 20 and 30 wt%) and bagasse fiber content (10, 20 and 30 wt%) were designed and produced. After the curing process, test samples were cut according to the sizes of ASTM standards. Fig.2.1 shows some of the moulds and the sample pieces.

Fig.2.1: Fabricated moulds and test specimens Page 21

International Journal of Engineering Research Volume No.3, Issue No.1, pp : 21-25

III. Mechanical Tests The samples of pre-fixed fiber content of produced hybrid fiber reinforced composites were investigated for their tensile, flexural and impact properties. Both tensile, flexural and impact strength tests were conducted for all the nine samples. Tensile Strength Test The tensile strength of the composites was measured with a universal testing machine in accordance with the ASTM D3039 procedure. The speed of the tensile testing machine is about 2mm/min. The tensile strength of all nine combinations is shown in Fig.3.1. Flexural Strength Test The flexural strength of the composites was also done by universal testing machine in accordance with the standard of ASTM D790. The speed of the machine is about 2mm/min. The

(ISSN:2319-6890)(online),2347-5013(print) 01 Jan. 2014 The testing results were tabulated for corresponding fiber weight ratio in Table 3.1. Table 3.1 Mechanical properties of composites A B Tensile Flexural Sample Coir Bagasse Strength Strength Identification (%) (%) (MPa) (MPa) S1 10 10 15.83 35.84 S2 20 10 22.13 42.64 S3 30 10 26.45 44.31 S4 10 20 17.69 37.36 S5 20 20 22.6 43.12 S6 30 20 23.42 44.2 S7 10 30 12.52 30.84 S8 20 30 16.83 34.18 S9 30 30 18.72 37.98

Impact Energy (J) 3.5 4.1 4.5 3.0 3.2 4.2 3.0 3.3 4.0

flexural strength of all nine combinations is shown in Fig.3.2. Impact Strength Test The izod impact test was conducted to find the impact energy in accordance with the standard of ASTM D256. The impact energy of all nine combinations is shown in Fig.3.3.

Fig.3.1: Effect of fiber parameters on tensile strength

IV. Factorial Design Method Factorial design is a systematic method that investigates the effects of two or more factors on the output response process. Each trail or replication of the experiment takes into account all the possible combinations of the varying levels of these factors. In this case, two factors (wt% of coir and wt% of bagasse fibers) are the parameters with three levels (-1,0,1) in each factor, so totally 3 x 3 = 9 runs(experiments) were conducted for studying the influence on the response of tensile, flexural and impact strengths. The running of factorial combinations and the mathematical interpretation of the output responses of the process to such combinations is the essence of factorial experiments. It allows an engineer to understand which factors affect the process most, so that improvements may be attained. Fig.4.1 shows the optimum fiber parameter values obtained from factorial design method for tensile, flexural and impact strengths.

Fig.3.2: Effect of fiber parameters on flexural strength

Fig.4.1: Optimum fiber parameter values obtained from factorial design method Fig.3.3: Effect of fiber parameters on impact strength IJER@2014

Page 22

International Journal of Engineering Research Volume No.3, Issue No.1, pp : 21-25

(ISSN:2319-6890)(online),2347-5013(print) 01 Jan. 2014

V. Analysis of Variance

VII. Scanning Electron Microscopy

ANOVA technique can be used to investigate any number of factors which are hypothesized or said to influence the dependent variable. This design consisted of two factors, each at three levels.

The Scanning Electron Microscopy testing was conducted on a tensile test specimen to find the fiber matrix interfacial adhesion. The SEM testing morphology images are as follows. The testing was conducted in various higher magnifications of 100µm, 50µm, 20µm and 10µm. The tensile testing specimens were used for testing.

ANOVA for Tensile Strength Test The list of degrees of freedom, sum of squares and mean square for tensile strength model are given in Table 5.1. The Model F-value of 32.18 implies the model is significant. There is only a 0.83% chance that a "Model F-Value" this large could occur due to noise. Values of "Prob > F" less than 0.0500 indicate model terms are significant.In this case A, B, B 2 are significant model terms. Values greater than 0.1000 indicate the model terms are not significant. ANOVA for Flexural Strength Test The list of degrees of freedom, sum of squares and mean square for flexural strength model are given in Table 5.2. The Model F-value of 31.56 implies the model is significant. There is only a 0.85% chance that a "Model F-Value" this large could occur due to noise. Values of "Prob > F" less than 0.0500 indicate model terms are significant. In this case A, B, B2 are significant model terms. Values greater than 0.1000 indicate the model terms are not significant.

The SEM images represented for coir and bagasse in tensile testing specimen are shown in Fig.7.1 & 7.2 respectively. From these images, it is cleared that there is no pull out holes on the specimens. Instead of that the breaking of fibers only found out. So, the bonding between fibers and polyester resin was extremely high. That bonding could not break up while tensile loading. Instead of pull out holes, the fiber breaking only occurred during the tensile loading. So, the interfacial bonding adhesion between the fiber and polymer matrix was considerably good while in tensile loading conditions.

ANOVA for Impact Test The list of degrees of freedom, sum of squares and mean square for impact strength model are given in Table 5.3. The Model F-value of 15.00 implies the model is significant. There is only a 2.47% chance that a "Model F-Value" this large could occur due to noise. Values of "Prob > F" less than 0.0500 indicate model terms are significant. In this case A, B are significant model terms. Values greater than 0.1000 indicate the model terms are not significant. Fig.7.1: SEM image for coir

VI. Non-Linear Regressive Analysis The mechanical properties such as tensile and flexural strength were modeled using second-order polynomial curve fitting equations using Design Expert statistical software. Equation (1) - (3) are the developed non-linear regression models of tensile strength (TS), flexural strength (FS) and impact energy (IE) respectively. TS = 0.07 + 1.16283 A + 0.94467 B - 0.01105 AB - 0.01415 A2 - 0.0249 B2 (1) FS = 18.43556 + 1.064 A + 1.308 B – 0.003325 AB 0.015583 A2 - 0.039283 B2 (2) IE = 4.62222 - 0.013333 A - 0.13667 B - 3.1225E-018 AB + 0.00167 A2 + 0.00267 B2 (3) IJER@2014

Fig.7.2: SEM image for bagasse

Page 23

International Journal of Engineering Research Volume No.3, Issue No.1, pp : 21-25

VIII. Conclusion Thus the comparison of tensile, flexural and impact strength for different combination of coir and bagasse fiber contents with polymer resin were done and the optimal mixing of fibers weight ratio were calculated for the effective tensile strength, flexural strength and the impact energy. In this present work, we found out that the 30% of coir fiber and 10% of bagasse fiber with 60% of polyester resin resulted the best values of tensile strength, flexural strength and impact energy i.e., 26.45 MPa, 44.31 MPa and 4.5 J. Here, the second-order polynomial curve fitting equations were modelled which predicts the values of tensile, flexural and impact strengths with various other combination of fibers contents with resin. From the SEM test, it is cleared that there is no pull out holes on the specimens. Instead of that the breaking of fibers only found out. Thus the bonding between fibers and polyester resin was extremely high.

Acknowledgement First and foremost we express our sincere thanks to our parents for their blessings in every step. We extend our heartfelt thanks to all our staff members and friends those who are contributing moral support and encouragement to do this work. We also thank all those who have directly involved or indirectly helped for the successful completion of this research work.

References i. N.S.M. El-Tayeb, 2008, A study on the potential of sugarcane fibers/polyestercomposite for tribological applications, Wear 265, pp. 223-235. ii. E. F. Cerqueira, C. A. R. P. Baptista, 2011. Mechanical behaviour of polypropylene reinforced sugarcane bagasse fibers composites, Procedia Engineering 10, pp. 2046

IJER@2014

(ISSN:2319-6890)(online),2347-5013(print) 01 Jan. 2014 iii. A Karthikeyan and K Balamurugan, 2012. Effect To Alkali Treatment And Fiber length On Impact Behavior Of Coir Fiber Reinforced Epoxy Composites. Journal of Scientific & Industrial Research 71, pp. 627. iv. S. Velumani, P. Navaneethakrishnan, S. Jayabal and D.S. Robinson Smart, 2013. Optimization of mechanical properties of non-woven short sisal fibre-reinforced vinyl ester composite using factorial design and GA method. Indian Academy of Sciences, Vol.36, pp. 575-583. v. R. Balasubramanian, K. Sankaranarayanasamy, 2010. Mathematical modelling and optimisation of laser welding of butt joints, Int. J. Computational Materials Science and Surface Engineering, Vol. 3, No. 4, pp. 321. vi. Tran Huu Nam, Shinji Ogihara (2011) ‘Effect of Alkali Treatment on Interfacial and Mechanical Properties of Coir Fiber Reinforced Poly(Butylene Succinate) Biodegradable Composites’ Composites: Part B 42, pp 1648–1656. vii. P.A. Sreekumar, Kuruvilla Joseph, G. Unnikrishnan, Sabu Thomas, 2007. A comparative study on mechanical properties of sisal-leaf fibre-reinforced polyester composites prepared by resin transfer and compression moulding techniques. Journal of Composites Science and Technology 67, pp. 453-461. viii. H. Ku, H. Wang, N. Pattarachaiyakoop (2011) ‘A Review on the Tensile Properties of Natural Fiber Reinforced Polymer Composites’ Composites: Part B 42, pp 856–873.

ix. Yung-Kuang Yang, Rong-Tai Yang, 2012, ‘Optimization of mechanical characteristics of short glass fiber and polytetrafluoroethylene reinforced polycarbonate composites using the neural network approach’, Expert Systems with Applications 39, pp. 3783. x. B. Balamugundan, L. Karhikeyan, 2012, ‘Multi character optimization during milling of friction stir processed glass fiber reinforced composites’, Procedia Engineering 38, pp. 1276.

xi. Douglas C. Montgomery., 5th Edition, Design and Analysis of Experiments, John wiley & Sons.

Page 24

International Journal of Engineering Research Volume No.3, Issue No.1, pp : 21-25

(ISSN:2319-6890)(online),2347-5013(print) 01 Jan. 2014

Table 5.1 ANOVA for tensile strength model Response 1 Tensile Strength ANOVA for Response Surface Quadratic Model Analysis of variance table [Partial sum of squares - Type III] p-value

Source

Sum of Squares

df

Mean square

F value

Model A-COIR B-BAGASSE AB4.88 A24.00

150.54 84.75 44.50 4.88 4.00

5 1 1 1 1

30.11 84.75 44.50 4.88 4.00

32.18 90.57 47.56 5.22 4.28

0.0083 0.0025 0.0062 0.1065 0.1304

B212.40 Residual Cor Total

12.40 2.81 153.35

1 3 8

12.40 0.94

13.25

0.0357

Prob > F significant

Table 5.2 ANOVA for flexural strength model Response 2 Flexural Strength ANOVA for Response Surface Quadratic Model Analysis of variance table [Partial sum of squares - Type III] p-value

Source

Sum of Squares

df

Mean square

F value

Model A-COIR B-BAGASSE AB A2

185.44 84.00 65.27 0.44 4.86

5 1 1 1 1

37.09 84.00 65.27 0.44 4.86

31.56 71.48 55.55 0.38 4.13

0.0085 0.0035 0.0050 0.5830 0.1350

B2 Residual Cor Total

30.86 3.53 188.96

1 3 8

30.86 1.18

26.26

0.0144

Prob > F significant

Table5.3 ANOVA for impact energy model Response 3 Impact Energy ANOVA for Response Surface Quadratic Model Analysis of variance table [Partial sum of squares - Type III] p-value

Sum of Squares

df

Mean square

F value

Model A-COIR B-BAGASSE AB A2

2.44 1.71 0.54 0.000 0.056

5 1 1 1 1

0.49 1.71 0.54 0.000 0.056

15.00 52.36 16.57 0.000 1.70

0.0247 0.0054 0.0268 1.000 0.2828

B2 Residual Cor Total

0.14 0.098 2.54

1 3 8

0.14 0.033

4.36

0.1279

Source

IJER@2014

Prob > F significant

Page 25

Advertisement

Read more

Similar to

Popular now

Just for you